Download presentation

Presentation is loading. Please wait.

Published byBrynn Newman Modified over 2 years ago

1
高温超導的量子磁通状態和相変 胡 暁 計算材料科学研究中心 物質・材料研究機構、日本筑波 hc/2e |||| B JsJs Vortex states and phase transitions in high-Tc superconductivity Xiao Hu National Institute for Materials Science, Tsukuba, Japan

2
Summary Outline Introduction Melting of flux line lattice in HTSC ♣ B || ab plane ♣ impacts of point defects ♣ B || c axis ab plane c axis

3
GL theory for superconductivity Superconductivity order parameter: e i GL free energy functional: =- ’(1-T/T c ) Two length scales : (i)Correlation length of SC order parameter: ~1/√(1-T/T c ) (ii) Penetration depth of magnetic field: ~1/√(1-T/T c ) GL number: (i) <<1(ii) >1(iii) >>1

4
MF phase diagram: two 2 nd order trs. |||| B JsJs Meissner phase Mixed phase Normal phase H T H c2 H c1 ♣ H c1 =ln 0 /4 2 ♣ H c2 = 0 /2 2 Flux quantization: hc/2e ♣ =( 0 /4 ) 2 lnk ♣ V(r)=2( 0 /4 ) 2 ln( /r) Broken symmetry: (i) U(1) gauge symmetry (ii) translational symmetry Self energy and repulsion of vortices: penetration of flux Type-II SC : >1/√2 Vortex & flux quantum in type-II SC

5
Extremely type-II SC: >> Layer structure & high anisotropy: Importance of thermal fluctuations Experimental observations pancake vortex ab plane c axis H.Safar et al. 1993 A.Schilling et al. 1997E.Zeldov et al. 1995 Vortex states in HTSC

6
(i)Elastic theory for flux lines: C 11 & C 44 & C 66 (ii) Renormalization group: -expansions Lack of a good theory for 1 st order transitions! + Lindemann criterion for melting physical but phenomenological =6-D=3>>1 difficult to control the RG flows Theoretical approaches

7
where defined on 3-dim grids of simple cubic lattice: unit length d Derivable from Ginzburg-Landau Lawrence-Doniach model degrees of freedom: A ◆◆◆ Superconductivity order parameter: e i 3D anisotropic, frustrated XY model

8
Extremely type-II superconductors: d v d v ~d √ f Vortex as topological singularity of phases: B |||| dvdv d Flux line Magnetic induction: B || c axis f=Bd 2 / 0 =1/25 A=-r×B/2=(-yB/2,xB/2,0) Vortex and flux line

9
System size: L xy =50, L z =40 Boundary condition: periodic in 3 directions Typical process of MC simulations : ◆ generate a random configuration of phase variables at a high T ◆ cool system according to the Metropolis scheme ♣ search lattice structure ♣ measure T dependence of quantities MC simulation steps: ◆ equilibriution: 50,000 sweeps ◆ measurement: 100,000 sweeps ◆ around the transition point: ~ 10 7 sweeps Anisotropy: 2 =10 Temperature skips: ◆ ◆ around T m : T=0.1J/k B T=0.001J/k B Monte Carlo simulations

10
To achieve equilibrium in reasonable time: To simulate the fluctuations sufficiently: A big system A small system Slow annealing Quick annealing We know the spatial and temporal scales only after the phenomenon is understood. A serious trade off! We don ’ t even know if the Hamiltonian is sufficient! Can call them approximations? We deal with Hamiltonian. Good computer! Good luck! Good physics! Simulation: theory or experiment?

11
Finite size scaling: C + ≈ 18.5k B C - ≈ 17.5k B C max ≈ 23k B Q ≈ 0.07k B T m T ≈ 0.008T m First order thermodynamic phase transition

12
Note | | is finite even for T>T m U(1) gauge symmetry is broken at T=T m Phase stiffness & conductance Normal to superconductivity transition

13
Eliminate possibilities of : disentangled flux-line liquid; supersolid Translational symmetry is also broken at T m. T

14
T~0 Abrikosov flux line lattice Flux line liquid ~ spaghetti T≥T m Real space snapshot

15
Mechanism of melting: FL entanglement

16
Clausuis-Clapeyron relation: Lindemann number: c L =0.18 Melting line: B liquid >B solid Same as water! Length scale: d Competition: Elastic energy Thermal fluc. B-T phase diagram: melting line

17
B=8T T m [K] T m [K] S[k B /vortex] B[G] simulation 81 81 0.55 0.55 0.19 0.19 experiment 79 79 0.4 0.4 0.25 0.25 YBCO: d=12 Å, ab (0)=1000 Å, =8, T c =92K, =100 by Schilling et al. BSCCO: d=15 Å, ab (0)=2000 Å, =150, T c =90K, =100 by Zeldov et al.B=160G T m [K] T m [K] S[k B /vortex] B[G] simulation 65 65 0.22 0.22 0.12 0.12 experiment 65 65 0.4 0.4 0.35 0.35 Ref. XH, S. Miyashita & M. Tachiki, PRL 79, p.3498 (1997); PRB 58, p.3438 (1998) Comparison with experiments

18
Q Phase transition under B || ab plane ? cf. B ||c axis: 2-dim symmetry in ab plane 1 st order melting For H=0 (1) <∞: 2 nd order transition in 3D XY universality class (2) =∞: KT transitions in decoupled layers translational symmetry along c axis is broken a priori Difficulty in experiments: high anisotropy requiring very accurate alignment of magnetic field with CuO 2 layers Intrinsic pinning of CuO 2 layer to Josephson vortices Phase transition for B || ab plane

19
Korshunov & Larkin, 1992Mikheev & Kolomeisky, 1991 There should be no decoupling, provided that Josephson vortices are confined by CuO 2 layers for T ≤ T d. Decoupling transition: T d SC transition: T c T c >T d r Hopping of Josephson flux line via a pancake pair Binding & unbinding of pancake pairs KT transition Blatter et al. 1991 Liquid → Smectic → Solid two-step freezing Balents & Nelson, 1994 Two 2 nd order transitions Theories

20
Magnetic field: B || y axis x c System size: # of flux lines = 240 Periodic boundary conditions Anisotropy: =8 A=(0,0,-xB) f=Bd 2 / 0 =1/32 L x *L y *L z =384d*200d*20d Details of Monte Carlo simulation

21
◆ ◆ Response to applied current I FpFp FLFL non-Ohmic resistivity I FLFL Ohmic resistivity f=1/32 =8 x ~ y c =0 intrinsic pinning cf. universal jump of helicity modulus at KT transition: k B T KT =2/ 1 st order phase transition

22
k c = /10dk x = /192d Structure of Josephson vortex lattice

23
k c = /10dk x = /192d １ 2 Melting of Josephson vortex lattice

24
2 nd order melting for large anisotropy Tricritical point: tc =9~10 @ f=1/32 ♣ f=1/25, 1/36 tc increases as f decreases f=1/32 Other parameters: ♣ =7,6,…1 for f=1/32 1 st order melting

25
Mechanism of the tricritical point Tricritical Point! Invariant unit cell for >8 at f=1/32 Balance of inter-vortex repulsions (2d) 2 =d 2 +(d/2f ) 2 For > tc, fluctuations along c axis are essentially suppressed by layers 1 2 3 MF theory for flux line lattice melting: 3 rd order terms exist for < tc Numerically, tc =16/√3≈ 9.24 @ f=1/32 Simulations give 9< tc <10 1 st order melting, as B|| c axis 2 nd order melting suppressed for > tc

26
Thermal excitations Ratio of collisions and hoppings Observation of hopping of Josephson flux lines at T

27
No 2 nd order phase transition, provided no hopping T c

28
Tricritical magnetic induction Ref. XH & M.Tachiki, PRL 85, p.2577 (2000) 1 st order melting 2 nd order melting Tricritical point T KT T B TcTc T KT ~0.89J/k B =8 d=12 Å B tc ≒ 50 Tesla YBCO BSCCO B tc ≒ 1.7 Tesla =150 d=15 Å B-T phase diagram for B||ab plane

29
1 st order melting 2 nd order melting Tricritical point T KT T B TcTc T KT ~0.89J/k B 2 nd order melting Competition: elastic vs. thermal commensuration effect Pinning effect of CuO 2 layers suppress c-axis fluctuations length scales: d & d Small B: B m ~ (k B T m /J) -2 × 0 / d 2 B m,ab /B m,c ~ tricritical point Large B: T m →T KT decoupled limit B-T phase diagram for B||ab plane

30
H p =- ∫ d D rV(r) (r) H el =c ∑ ij u i u j u i =x i -R i 0 (r)= ∑ i (r-R i 0 -u i ) u(R a )-u(0)~a: lattice spacing a el =c(a/R a ) 2 R a D =cR a D-2 a 2 p =-VR a D/2 0 R a ~a[c 2 a D /(V 0 ) 2 ] 1/(4-D) Arbitrarily weak disorders destroy lattice order for D<4! “ Linearized ” Larkin model B(r) ≡ ‹ [u(r)-u(0)] 2 › ~(r/R a ) 4-D C(r)~exp(-B)~exp[-(r/R a ) 4-D ] Larkin length Similar arguments in other systems such as CDW etc. Impacts of point defects: Larkin theory

31
RaRa Dislocation Gauge glass: H= ∑ ij cos( i - j -A ij ) No positional order in D=3 liquid Vortex glass T H Physics: for a lattice of flux lines, one line does not have to make displacement much larger than a to pass through a particularly favorable region of disorders, because of periodicity. cf. a single flux line Asymptotic Alnr B r RaRa RcRc Larkin Random manifold r 2 C(r)~1/r Quasi LRO! Impacts of point defects

32
Q How many phases? Characters of phase transitions? How to understand them in a unified scheme? Bragg glass B T vortex liquid 1 st order Q: phase? Q: phase transition? Q: 1 st order? Bragg glass quasi long-range correlation free of dislocations Bragg glass melting thermal fluctuations intensity of pins Competitions: elasticthermalpinning Effects of point pins: B||c axis

33
interaction J interaction (1- )J with probability p Details of our approach filling factor: f=1/25 anisotropy parameter: =20 system size: L xy =50, L z =40 s.c. lattice & p.b.c. density of point defects: p=0.003 MC sweeps: equilibriution: 4~8*10 7 measurement: 2~4*10 7 Model with point defects

34
Ref. Y. Nonomura & XH: PRL 86, p.5140 (2001) -T phase diagram

35
Same as the melting of Abrikosov lattice Thermal melting of Bragg glass

36
Structure factors Bragg glass Vortex liquid Bragg glass: as perfect as a lattice Global minimumEnergy landscapeDynamics

37
● 1 st order phase transition cancellation ◆◆ pinning energyelastic energy ● phase boundary almost parallel to T axis e[J] Defect-induced melting of Bragg glass

38
● 1 st order phase transition at T sl ● SC achieved only at T=T g (

39
● sharp jump in the density of dislocations at T sl Ref. Kierfeld & Vinokur, 2000 Liquid to slush transition

40
● Bouquet et al. Nature 411, p.448 (2001) ● a step-like anomaly in C left ● no vortex loop blowout ● -function peak in C ● same in jump of disl. density suppressed above ≈ 0.15 critical endpoint! Ref. Kierfeld & Vinokur, 2000 high fields Trace of BrG melting Crossover?! Like liquid-gas line of water! Point pins create attractive force! Critical endpoint and beyond

41
Summary Melting of flux line lattice in HTSC Computer simulations B || c axis: 1 st order, FLL to entangled liquid B || ab plane: tricritical point Impacts of point defects under B || c axis Belong to the category of theory Try to break the frontier! Try to go beyond theory! New concept New paradigm

Similar presentations

Presentation is loading. Please wait....

OK

Superconductivity in Zigzag CuO Chains

Superconductivity in Zigzag CuO Chains

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on earth dam design Free download ppt on lost city of atlantis Ppt on sports day hs Download ppt on indus valley civilization art Ppt on conceptual art history Ppt on eid festival india Ppt on resistance temperature detector failures Ppt on indian road signs Ppt on aerobics steps Ppt on census 2001 kerala